Research Article | Open Access
Rafal Kruszynski, Tomasz Sieranski, Bartlomiej Lewinski, Agata Trzesowska-Kruszynska, Ewelina Czubacka, "The Novel Polymorphic Form of Bis(3,5,7-triaza-1-azoniatricyclodecane) bis(-oxo)-tris(-oxo)-nonakis(-oxo)-nonaaqua-decaoxo-hepta-molybdenum-di-zinc(II) dihydrate, Synthesis, and Properties", International Journal of Inorganic Chemistry, vol. 2012, Article ID 516832, 7 pages, 2012. https://doi.org/10.1155/2012/516832
The Novel Polymorphic Form of Bis(3,5,7-triaza-1-azoniatricyclodecane) bis(-oxo)-tris(-oxo)-nonakis(-oxo)-nonaaqua-decaoxo-hepta-molybdenum-di-zinc(II) dihydrate, Synthesis, and Properties
The reaction of molybdophosphoric acid with zinc carbonate followed by addition of hmta leads to formation of a triclinic polymorph of bis(3,5,7-triaza-1-azoniatricyclodecane) bis(-oxo)-tris(-oxo)-nonakis(-oxo)-nonaaqua-decaoxo-hepta-molybdenum-di-zinc(II) dihydrate in a one pot simple reaction. The obtained compound has been characterised by IR, UV-Vis spectroscopy, elemental analysis, and X-ray crystallography. A detailed comparison between both polymorphic forms: triclinic Å, Å, Å, , , , and Å3 and monoclinic Å, Å, Å, , , , and Å3 was performed. The influence of the synthesis procedure on polymorph formation was described.
The coordination chemistry of zinc is a field of growing interest from various viewpoints. The attention of scientists concentrates on synthetic aspects, structural, physicochemical properties, and reactivity of zinc compounds, as well as on their potential applications such as the development of catalysts (C–C bond formation reactions , carbon dioxide activation [2–4], etc.). Zinc complexes compounds are widely studied as biological mimics [5–7]. Zinc is an essential element for humans and is homeostatically regulated in the body. It has an important role in protein synthesis, and it is also a cofactor for many enzymes regulating cell growth and hormone levels, including regulation of gene transcription and growth factor metabolism . Moreover, the mean zinc and lead concentrations in the human body correlate with the degree of urbanization and industrialization [9, 10].
Transition metal oxides such as molybdenum oxides are used in many industrial applications and have gained an interest from both technological and scientific points of view [11–15]. The main fields of industrial applications are catalysis, sorption, energy storage, molecular electronics, optical materials, and ceramics [16, 17]. Molybdenum oxides are an interesting example of this group of compounds and have a great industrial interest due to their optical and electronic properties. In fact, these transition metal oxides can be switched between two different optical states by photochromic, thermochromic, or electrochromic means . Compounds that contain molybdenum oxides substructures modified by organonitrogen ligands were classified as a fifth class of oxides in which organic materials play a significant structural role . Taking the above into consideration, there is a need for synthesis and investigations of new molybdenum cluster compounds. These compounds, containing additionally zinc cations, may possess interesting biological properties, joining in one compound the benefits of both a molybdenum cluster and zinc ions.
Hexamethylenetetraamine (hmta) is an interesting ligand forming a diversity of complex compounds. It is used in pharmaceutical and in chemical industries as an intermediate material . Since the discovery of hmta, over a century ago, an enormous number of its salts, molecular adducts, and coordination complexes have been reported in the literature . Hmta is a potentially tetradentate ligand, universally used for the construction of supramolecular arrays with various hmta coordination modes utilising from one to four nitrogen atoms . Additionally, the hmta can be located in outer coordination sphere and influence the inner coordination sphere of metals by supramolecular bond array.
Polymorphism is a commonly known phenomenon [22–26]. Polymorphic transitions influence many properties of a compound, for example, physical stability, chemical stability, and manufacturability or in the case of drugs, can for example change the kinetics of oral absorption. Relatively small changes in crystal packing may lead to significant differences in the crystal packing density and other properties of polymorphs [27, 28].
Compounds containing many independent molecules in the unit cell of inorganic-organic compounds seem to be currently a subject of great interest both for pure science and for its industrial consequences, especially for pharmaceutical production and technical applications, as they can be considered as “locked in” compounds formed too early in crystallization processes and thus differing from the thermodynamically most stable structures [29, 30]. Such “locked in” compounds are a relatively good source of the new polymorphic forms of known compounds . In the recent literature, it is observed an increasing amount of reports dedicated to the development of new compounds possessing and to the study of their properties [31, 32].
While searching and studying polymorphic forms of compounds possessing useful properties, a new polymorph of zinc complex compound containing hexamethylenetetraamine and a molybdenum cluster was obtained and is presented here.
2.1.1. Preparation of bis(-oxo)-tris(-oxo)-nonakis(-oxo)-nonaaqua-decaoxo-hepta-molybdenum-di-zinc(II)
The zinc (II) carbonate (0.003 mol, 0.3762 g) was suspended in solution of dodecamolybdophosphoric acid (H3PO4·12MoO3·24H2O, 0.001 mol, 2.2652 g) in 30 cm3 of water. The suspension was stirred on a magnetic stirrer until pH of mixture was 7.0 (about 3 hours). Within this time, the precipitation of non-soluble zinc (II) phosphate (V) (Zn3(PO4)2) was observed. Then, the mixture was filtered to remove unreacted excess of zinc carbonate and deposit of zinc (II) phosphate (V). The residue on the filter was washed three times with 5 cm3 of cold water. The last filtrate showed no presence of molybdate (VI) on the basis of test with hydrogen peroxide in acidic environment .
2.1.2. Preparation of the Compound 1
The solution of bis(-oxo)-tris(-oxo)-nonakis(-oxo)-nonaaqua-decaoxo-hepta-molybdenum-di-zinc(II) obtained according to Section 2.1.1. was mixed with solution of hexamethylenetetramine (hmta, 0.001 mol, 0.1402 g in 10 cm3 of water). After six weeks of crystallization at 21–23°C the light green crystals were obtained and separated from the solution.
2.2. Crystal Structure Determination
Light green rectangular prism shape crystal was mounted on a KM-4-CCD automatic diffractometer equipped with CCD detector and used for data collection. X-ray intensity data were collected with graphite monochromated radiation ( Å) at temperature 291.0(3) K, with scan mode. 10 seconds exposure time was used and reflections inside Ewald sphere were collected up to . The unit cell parameters were determined from least-squares refinement of the setting angles of the 5034 strongest reflections. Details concerning crystal data and refinement are given in Table 1. Examination of reflections on two reference frames monitored after each 20 frames measured showed no loss of the intensity during whole measurement. Lorentz, polarization, and numerical absorption  corrections were applied. The structure was solved by direct methods. All the nonhydrogen atoms were refined anisotropically using full-matrix, least-squares technique on . The carbon-bonded hydrogen atoms were set in calculated position after four cycles of anisotropic refinement and refined as “riding” on the adjacent atom with individual isotropic displacement factor equal 1.2 times of the value of equivalent displacement factor of the patent carbon atoms. Due to flattening of difference Fourier syntheses, the oxygen-bonded hydrogen atoms could not be found. The hydrogen atom positions were idealised after each cycle of refinement. The SHELXS97, SHELXL97, and SHELXTL  programs were used for all the calculations. Atomic scattering factors were those incorporated in the computer programs.
2.3. Other Measurements
Elemental analysis was carried out using Vario EL III CHNOS elemental analyzer (C, H, N, O). Molybdenum (VI) content was determined by polarographic analysis in presence of EDTA  in mineralized sample. Zinc (II) content was determined by complexometric titration with EDTA used as a complexing agent . IR spectra of the samples in the form of KBr pellets were recorded on a Nicolet Magna 560 spectrophotometer in the spectral range 4000–400 cm−1. The UV-VIS spectra were recorded on Jasco V-660 spectrophotometer, in transmission mode, for solid samples pressed between two quartz plates. The thermal analysis was carried out in a TG/DTA-SETSYS-16/18 thermoanalyser coupled with thermostar (Balzers) mass spectrometer. The sample was heated in corundum crucibles up to 1000°C at a heating rate 2°C/min in air atmosphere. The products of the decomposition process were calculated from TG curves, and the temperature ranges were determined by means of thermoanalyser data processing module . The compound density was determined by Berman density torsion balance. Elemental analysis for 1 [Calculated/Found (%)] C12H48Mo7N8O35Zn2, C 8.61/8.58; H 2.9/3.00; O 33.61/33.01; Mo 40.32/40.58; N 6.57/6.58; Zn 7.99/7.90.
3. Results and Discussion
The bis(3,5,7-triaza-1-azoniatricyclo[126.96.36.199,7]decane) bis(-oxo)-tris(-oxo)-nonakis(-oxo)-nonaaqua-decaoxo-hepta-molybdenum-di-zinc(II) dihydrate was previously obtained in the monoclinic form (1a) (Herman-Maugin space group) , and the presented polymorph (1) adopts the triclinic symmetry ( space group) with doubled content of the unit cell ( and , resp., for (1a) and (1)). The only structural difference between both polymorphic forms is the crystal net symmetry (Figure 1), but it must be mentioned that the overall molecules arrangement in the crystal net is similar in both polymorphs. Inspection of the crystal nets of 1a and 1 shows that the molecules occupy the same sites of the nets (Figure 1), but they are slightly rotated. Such rotation in 1 leads to motifs which do not reproduce the periodicity observed in 1a (the neighbouring molecules of 1 are connected only by pseudosymmetry elements, and some atoms deviate up to about 5% from the position originating from the symmetry elements present in 1a). The molecular geometry of the molecules is the same (in the range of experimental error) in 1 and 1a (See Supplementary Table 1 in Supplementary Material available online at http://dx.doi.org/10.1155/2012/516832).
The title compound was synthesized in a two-step synthesis starting from molybdophosphoric acid and zinc carbonate, with addition of hmta at the second step. The formation of molybdenum clusters originates from a protonation of molybdate anions by a strong mineral acid for example, hydrochloric acid . In the case of 1, the clustering was attained in situ by protons from molybdophosphoric acid. This synthesis procedure is simpler than that described earlier , because there is no necessity to adjust pH by adding the acid solution, but it must be noted that it leads to formation of a polymorphic form in the solid state. Formation of the bond between nonmetal and nitrogen atoms is not possible in a solution at low pH  and also at neutral pH (as it was found for compound 1).
The infrared spectrum of 1 is consistent with the presence of the molybdenum oxide cluster and hmta ligand. The weak peak at 769 cm−1 is attributed to the vibration of MoO bonds similarly to the oscillator observed in molybdenum (VI) oxide, but it is slightly shifted to higher frequencies due to utilisation of terminal oxygen atoms lone pairs into O→Mo interactions in molybdenum (VI) oxide and thus weakening of the oscillators in that compound [39, 40]. The sharp peak at 896 cm−1 is attributed to the Mo=O bonds, which is a characteristic for the symmetric and asymmetric stretches of the MoO cis-dioxo group [38, 40–42]. The very week band at 962 cm−1 is assigned to the stretching vibrations of bonds of Mo–O–Mo group [43–46] as well as to the vibrations of the double bond of the Mo=O group . This band can also suggest the presence of molybdenum in the lower oxidation state, that is, Mo5+ [39, 40] but in the studied compound, it is impossible due to stoichiometry. The absorption bands observed at 1636 and 3480 cm−1 can be attributed to the bending vibrations of O–H bonds of zinc-coordinated water molecules . In 1, all IR absorption maxima (typical for hmta molecules existing in the outer coordination sphere) are also observed (Table 2). The IR spectrum of 1 is more complex than that of 1a  (Table 2), and some oscillators have different energy in each compound. The peak attributed to vibrations of OH bonds of compound 1 water molecules (at 1636 cm−1) is shifted to lower frequencies (about 22 cm−1) in comparison to 1a, and the analogous vibrations at 3480 cm−1 are shifted to higher frequencies (about 30 cm−1), which originate from different intermolecular interactions in both compounds. In both polymorphic forms, bands attributed to MoO bonds and peaks assigned to hmta are present. They exist at the same wave numbers, but some vibrations observed in the IR spectrum of 1 are not reported (however, they are probably observed) in case of compound 1a (including strong bands at 664.3, 831.8, 2993.7, and 3005.8 cm−1).
|Vibrations symbols: vw: very weak, w: weak, m: medium strength, s: strong, vs: very strong, bb: broad band, : stretching, δ: bending, τ: wagging, ω: twisting, ρ: rocking, σ: scissoring, s: symmetric, and as: asymmetric.|
The solid state UV-Vis spectrum of compound 1 shows maxima at 243, 299, 536, 590, and 749 nm. The first two bands are also detected in the UV-Vis diffuse reflectance spectrum of molybdate clusters [47, 48]. The band at 243 nm is attributed to electronic transitions in tetrahedral molybdate, while the band at 299 nm is assigned to electronic transitions in Mo–O–Mo bridge bond existing between two octahedral metal atoms of molybdate . Both these absorption maxima exist in electronic spectra of molybdenum (VI) oxide (this oxide possesses a total of four absorption maxima in UV-VIS spectrum at 217, 245, 326, and 620 nm), but it is worth noticing that in 1, the second one is distinctly blue shifted (about 27 nm) in comparison to molybdenum (VI) oxide . The first broad band (243 nm) is assigned to transitions, and its shape and position are the consequence of the presence of many double Mo=O bonds in the compound 1. The second band (299 nm) can be attributed to the transitions and it is a characteristic of oxygen atoms bonded to metal atoms by a double bond . The above-mentioned blue shift originates from enlarged energy gap between and orbitals caused by localising of orbitals on oxygen atoms of 1 (in molybdenum (VI) oxide, these orbitals are partially utilised for creation of O→Mo interactions, thus they have larger energy). The two absorption maxima (at 217 and 620 nm) existing in the UV-VIS spectrum of molybdenum (VI) oxide are not observed in 1. The absorption maximum at 217 nm (assigned to electron transitions) is blue shifted to the vacuum ultraviolet region (because the M=O bonds in molybdenum (VI) oxide are longer and thus weaker than those ones existing in compound 1, this increases the energy gap between the and orbitals). Due to the impossibility of total removing of atmospheric nitrogen from solid samples, such shifted absorption maxima could not be identified in the case of the current compound. The visible region absorption of molybdenum (VI) oxide with absorption maximum at 620 nm (responsible for the yellow-green colour of the compound) is absent in 1, and it is replaced by three absorption maxima (two strong at 536, 590 nm and one medium strength at 749 nm) responsible for the green colour of crystals of 1.
The thermal decomposition of the investigated complexes is a gradual process. According to TG and DTG curves, compound 1 decomposes by the same scheme as observed for 1a , but the DTA curve obtained for compound 1 shows a distinctly smaller endothermic peak during the water evolution process accompanied by a very small exothermic peak, not observed in 1a. Thus, it can be supposed that during the first step of thermal degradation, the differences between the polymorph disappear, and the resulting anhydrous compounds have the same structure.
The reaction of molybdophosphoric acid with zinc carbonate followed by addition of hmta leads to formation of a triclinic polymorph of bis(3,5,7-triaza-1-azoniatricyclo[188.8.131.52,7]decane) bis(-oxo)-tris(-oxo)-nonakis(-oxo)-nonaaqua-decaoxo-hepta-molybdenum-di-zinc(II) dihydrate in a one pot simple reaction. Some differences were observed between the properties of the two polymorph, for example, some IR spectral bands observed in 1 are shifted in comparison to 1a, and some bands are unreported or absent in the spectrum of 1. During thermal decomposition, different effects were observed. In addition, 1 is slightly denser than 1a (about 0.01 Mg/m3).
Supplementary Table 1. Selected bond lengths and interbond angles of 1 and 1a (Å, °).
- T. Darbre and M. Machuqueiro, “Zn-proline catalyzed direct aldol reaction in aqueous media,” Chemical Communications, vol. 15, p. 1090, 2003.
- D. J. Darensbourg, J. R. Wildeson, and J. C. Yarbrough, “Solid-state structures of zinc(II) benzoate complexes. Catalyst precursors for the coupling of carbon dioxide and epoxides,” Inorganic Chemistry, vol. 41, no. 4, pp. 973–980, 2002.
- Y. Kawakami, K. Tajima, and T. Tsuruta, “Three-membered ring formation-IV. Selective syntheses of halogenocyclopropanedicarboxylic esters possessing different alcohol residues,” Tetrahedron, vol. 29, no. 9, pp. 1179–1183, 1973.
- D. J. Darensbourg and M. S. Zimmer, “Copolymerization and terpolymerization of CO2 and epoxides using a soluble zinc crotonate catalyst precursor,” Macromolecules, vol. 32, no. 7, pp. 2137–2140, 1999.
- B.-H. Ye, X.-Y. Li, I. D. Williams, and X.-M. Chen, “Synthesis and structural characterization of di- and tetranuclear zinc complexes with phenolate and carboxylate bridges. Correlations between 13C NMR chemical shifts and carboxylate binding modes,” Inorganic Chemistry, vol. 41, no. 24, pp. 6426–6431, 2002.
- B. Singh, J. R. Long, F. Fabrizi De Biani, D. Gatteschi, and P. Stavropoulos, “Synthesis, reactivity, and catalytic behavior of iron/zinc-containing species involved in oxidation of hydrocarbons under Gif-type conditions,” Journal of the American Chemical Society, vol. 119, no. 30, pp. 7030–7047, 1997.
- G. Parkin, “Synthetic analogues relevant to the structure and function of zinc enzymes,” Chemical Reviews, vol. 104, no. 2, pp. 699–767, 2004.
- J. Brandão-Neto, V. Stefan, B. B. Mendonça, W. Bloise, and A. V. B. Castro, “The essential role of zinc in growth,” Nutrition Research, vol. 15, no. 3, pp. 335–358, 1995.
- G. Fosse and N. P. B. Justesen, “Lead in deciduous teeth of Norwegian children,” Archives of Environmental Health, vol. 33, no. 4, pp. 166–175, 1978.
- G. Fosse and N. P.B. Justesen, “Zinc and copper in deciduous teeth of Norwegian children,” International Journal of Environmental Studies, vol. 13, no. 1, pp. 19–34, 1978.
- A. F. Wells, Structural Inorganic Chemistry, Oxford University Press, Oxford, UK, 1975.
- N. N. Greenwood and A. Earnshaw, Chemistry of the Elements, Pergamon Press, New York, NY, USA, 1984.
- G. E. Buono-Core, G. Cabello, A. H. Klahn et al., “Growth and characterization of molybdenum oxide thin films prepared by photochemical metal-organic deposition (PMOD),” Polyhedron, vol. 29, no. 6, pp. 1551–1554, 2010.
- K. Bange, “Colouration of tungsten oxide films: a model for optically active coatings,” Solar Energy Materials and Solar Cells, vol. 58, no. 1, pp. 1–131, 1999.
- A. Bouzidi, N. Benramdane, H. Tabet-Derraz, C. Mathieu, B. Khelifa, and R. Desfeux, “Effect of substrate temperature on the structural and optical properties of MoO3 thin films prepared by spray pyrolysis technique,” Materials Science and Engineering B, vol. 97, no. 1, pp. 5–8, 2003.
- A. K. Cheetham, “Advanced inorganic materials: an open horizon,” Science, vol. 264, no. 5160, pp. 794–795, 1994.
- P. A. Cox, Transition Metal Oxides, Clarendon Press, Oxford, UK, 1995.
- P. J. Hagrman and J. Zubieta, “Solid-state coordination chemistry of metal oxides: hydrothermal synthesis and structural characterization of o-phenanthroline-ligated copper- and zinc-molybdenum oxides,” Inorganic Chemistry, vol. 38, no. 20, pp. 4480–4485, 1999.
- A. Alamdari and F. Tabkhi, “Kinetics of hexamine crystallization in industrial scale,” Chemical Engineering and Processing, vol. 43, no. 7, pp. 803–810, 2004.
- J. Altpeter, Das Hexamethylentetramin und Seine Verwendung, Knapp, 1931.
- M. Svensson, L.A. Bengtsson-kloo, and H. Stegemann, “(Hexamethylenetetramine)diiodomercury(II), HgI2.hmt,” Acta Crystallographica Section C, vol. 51, pp. 2289–2292, 1995.
- D. E. Bugay, “Characterization of the solid-state: spectroscopic techniques,” Advanced Drug Delivery Reviews, vol. 48, no. 1, pp. 43–65, 2001.
- G. A. Stephenson, R. A. Forbes, and S. M. Reutzel-Edens, “Characterization of the solid state: quantitative issues,” Advanced Drug Delivery Reviews, vol. 48, no. 1, pp. 67–90, 2001.
- D. J. W. Grant and H. Brittain, Eds., Polymorphism in Pharmaceutical Sciences, Drugs and the Pharmaceutical Sciences, Marcel Dekker, New York, NY, USA, 1999.
- M. J. Pikal and H. Brittain, Eds., Polymorphism in Pharmaceutical Sciences, Drugs and the Pharmaceutical Sciences, Marcel Dekker, New York, NY, USA, 1999.
- S. R. Byrn, R. R. Pfeiffer, and J. G. Stowell, Solid State Chemistry of Drugs, SSCI Incorporation, West Lafayette, Ind, USA, 2nd edition, 1999.
- D. Singhal and W. Curatolo, “Drug polymorphism and dosage form design: a practical perspective,” Advanced Drug Delivery Reviews, vol. 56, no. 3, pp. 335–347, 2004.
- J. Bernstein, J. D. Dunitz, and A. Gavezzotti, “Polymorphic perversity: crystal structures with many symmetry-independent molecules in the unit cell,” Crystal Growth and Design, vol. 8, no. 6, pp. 2011–2018, 2008.
- G. S. Nichol and W. Clegg, “Further thoughts on crystal structures with : analysis of single-crystal structures determined using X-ray synchrotron and neutron radiation in the Cambridge Structural Database,” CrystEngComm, vol. 9, no. 10, pp. 959–960, 2007.
- S. Aitipamula, G. R. Desiraju, M. Jaskólski, A. Nangia, and R. Thaimattam, “Multiple molecules in the crystallographic asymmetric unit. Self host-guest and doubly interpenetrated hydrogen bond networks in a pair of keto-bisphenols,” CrystEngComm, vol. 5, pp. 447–450, 2003.
- R. Bishop and M. L. Scudder, “Multiple molecules in the asymmetric unit () and the formation of false conglomerate crystal structures,” Crystal Growth and Design, vol. 9, no. 6, pp. 2890–2894, 2009.
- K. M. Anderson, A. E. Goeta, and J. W. Steed, “Supramolecular synthon frustration leads to crystal structures with Z′ > 1,” Crystal Growth and Design, vol. 8, no. 7, pp. 2517–2524, 2008.
- J. Minczewski and Z. Marczenko, Chemia Analityczna (eng. Analytical Chemistry), vol. 1, PWN, Warsaw, Poland, 1985.
- X-RED. Version 1.18. STOE & Cie GmbH, Darmstadt, Germany, 1999.
- G. M. Sheldrick, “A short history of SHELX,” Acta Crystallographica, vol. A64, no. 13, pp. 112–122, 2008.
- F. J. Welcher, Analityczne Zastosowanie Kwasu Wersenowego (eng. The Analytical Uses of Etylenediamineteraacetic Acid), WNT, Warsaw, Poland, 1963.
- Data Processing Module. Copyright © 1994–1998 SETARAM—FRANCE, Version 1.4.
- T. Arumuganathan, A. Srinivasarao, T. V. Kumar, and S. K. Das, “Two different zinc(II)-aqua complexes held up by a metal-oxide based support: synthesis, crystal structure and catalytic activity of [HMTAH] 2[Zn(H2O)5Zn(H2O)4Mo7O24]·2H2O (HMTAH = protonated hexamethylenetetramine),” Journal of Chemical Sciences, vol. 120, no. 1, pp. 95–103, 2008.
- T. He and J. Yao, “Photochromism of molybdenum oxide,” Journal of Photochemistry and Photobiology C, vol. 4, pp. 125–143, 2003.
- M. Ainwar, C. A. Hogarth, and C. R. Theocharis, “A study of the infrared absorption spectra of thin amorphous films of molybdenum trioxide,” Journal of Materials Science, vol. 24, no. 7, pp. 2387–2390, 1989.
- Z.-H. Zhou, H.-L. Wan, and K.-R. Tsai, “Molybdenum(VI) complex with citric acid: synthesis and structural characterization of 1 : 1 ratio citrato molybdate K2Na4[(MoO2)2O(cit)2]·5H2O,” Polyhedron, vol. 16, no. 1, pp. 75–79, 1997.
- C. G. Barraclough, J. Lewis, and R. S. Nyholm, “The stretching frequencies of metal-oxygen double bonds,” Journal of the Chemical Society, pp. 3552–3555, 1959.
- E. Guibal, C. Milot, O. Eterradossi, C. Gauffier, and A. Domard, “Study of molybdate ion sorption on chitosan gel beads by different spectrometric analyses,” International Journal of Biological Macromolecules, vol. 24, no. 1, pp. 49–59, 1999.
- R. A. A. Muzzarelli, Chitin, Pergamon Press, Oxford, UK, 1977.
- M. M. Miller and D. C. Sherrington, “Alkene epoxidations catalyzed by Mo(VI) supported on imidazole-containing polymers. I. Synthesis, characterization, and activity of catalysts in the epoxidation of cyclohexene,” Journal of Catalysis, vol. 152, no. 2, pp. 368–376, 1995.
- R. A. Nyquist and R. O. Kagel, Infrared Spectra of Inorganic Compounds (3800–45 cm-1), Academic Press, London, UK, 1971.
- M. Fournier, C. Louis, M. Che, P. Chaquin, and D. Masure, “Polyoxometallates as models for oxide catalysts. Part I. An UV-visible reflectance study of polyoxomolybdates: influence of polyhedra arrangement on the electronic transitions and comparison with supported molybdenum catalysts,” Journal of Catalysis, vol. 119, no. 2, pp. 400–414, 1989.
- G. Xiong, C. Li, Z. Feng, P. Ying, Q. Xin, and J. Liu, “Surface coordination structure of molybdate with extremely low loading on γ-alumina characterized by UV resonance Raman spectroscopy,” Journal of Catalysis, vol. 186, no. 1, pp. 234–237, 1999.
- T. Nowicka-Jankowska, UV-VIS Spectrophotometry in Chemical Analysis, PWN, Warszawa, Poland, 1988.
- J. O. Jensen, “Vibrational frequencies and structural determinations of hexamethylenetetraamine,” Spectrochimica Acta—Part A, vol. 58, no. 7, pp. 1347–1364, 2002.
- M. P. Bernstein, S. A. Sandford, L. J. Allamandola, and S. Chang, “Infrared spectrum of matrix-isolated hexamethylenetetramine in Ar and H2O at cryogenic temperatures,” Journal of Physical Chemistry, vol. 98, no. 47, pp. 12206–12210, 1994.
Copyright © 2012 Rafal Kruszynski et al. This is an open access article distributed under the Creative Commons Attribution License, which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.